Science of Welding Steel
|The General Problems|
|In this module I look cursorily (very!) on the art and science of liquid or fusion welding of steel. It has to be superficial and sketchy because there is no other way to treat this monstrously huge and complex topic in just a few pages. Moreover, I have never in my life welded anything myself.|
|I have looked at welding before in this Hyperscript:|
|There are many ways of fusion
welding. Here I restrict myself to "electrical" or
arc welding. Essentially you draw a powerful
electric discharge, an arc, between a
welding electrode and the metals to be welded. When we weld, we liquefy
surface-near regions of the two pieces of the metal to be welded and parts of
the electrode we use for arc welding. Generally we try to melt as little as
possible of the materials to be welded, having mostly liquid electrode material
in the resulting mix. The liquid flows into the region to be joined and
solidifies with a cooling rate that tends to be rather large. Why? First, the
melted volume is not so large so it has a large surface to volume ratio.
Second, most of the surface / interface is in contact with a good heat
conductor - the steel to be welded.
In a first approximation you must expect that the microstructure of the solidified weld seam will be similar to that obtained by casting the composition, followed by rapid cooling. And now you have the first problem with welding:
|That is not necessarily bad. If your weld seam
has a higher yield strength but smaller ductility than the bulk material, it
won't matter much if there is no need for further deformation. However, if
major stress builds up in the product later, like in a car accident or
here, the steel
will now come apart at the weld seams. Of course, the unavoidable
encountered during cooling must not exceed some critical limits in your weld
seam or cracking might occur right away,.
If your weld seam has a lower yield strength than the bulk material .... you can figure that out yourself.
|What compounds the problem is that solidification may start from both solid sides, with the center of the weld line solidifying last. Since the solid-liquid interface sweeps impurity atoms along because of segregation effects, the center of the weld is enriched with impurities that have a large effective segregation coefficient, and thus is possibly rather dirty - and then weak!|
|You can counter the difference in microstructure to some extent by choosing an electrode with optimal compositions (not necessarily fully identical to that of the steel to be welded) and countless tricks I can't go into (mostly because I don't know them).|
|The difference in the microstructure between the bulk material and the solidified materials is just the first problem. The second problem stems from the different microstructure in the Heat Affected Zone or HAZ. That is the area next to the formerly liquid parts that did not liquefy but still got rather hot. If you think that the HAZ cannot possibly be a bigger problem than the microstructure of the liquid part, think again.|
|The third problem results because (liquid) welding invariably produces major thermal gradients. In other words: the temperature changes enormously over small distances. Thermal gradients invariably cause stress until they disappear, and stress causes problems up to and including fracture.|
|Those are the obvious problems. The not-so-obvious ones result from the fact that you might get all kinds of unwanted stuff into the molten part: Oxygen and nitrogen from the air, stuff from the flux you use to prevent that, and in particular hydrogen from the welding process itself (see below). Since the liquefied part is vigorously stirred by all kinds of processes - you have a tremendous power density, after all - whisking in gases is easy and always detrimental.|
|There is little choice: you must protect the
liquefied part from direct contact with the air. This is where all those
"tricks" come in, and where welding turns into an art. In essence you
blow non-reactive gases over the liquefied part or even a liquid flux that
hopefully does not do anything bad to the steel. I'll give examples of that
It is not surprising that welding wasn't used right away when the age of steel started around 1850. It had to wait until 1920 or so before it was developed to a level where it could push steel technology to unprecedented heights. So, before I go briefly through the various problems encountered in welding, let's get one thing right:
|A Few Words to Welding Hardware|
|Welding for quite some time was mainly "flame" torch welding". Acetylene (C2H5) and oxygen from two high pressure cylinders are fed to a torch or blow pipe and ignited. The temperature in the flame is hot enough to melt iron and steel and thus allowed cutting and / or welding - provided you knew what you were doing and didn't set yourself and everything else on fire.|
|Torches are still used for cutting but rarely for welding anymore. That is now done by a plethora of methods, most of which use electricity in one form or other to supply the energy density necessary. Here I will only look very superficially on arc welding.|
|In essence, you draw an electrical
discharge - an arc - between the material to be welded and a welding electrode.
The arc is confined to a region scaling with the diameter of the electrode and
thus might cover an area of some 10 mm2. The power delivered is
voltage times current. With voltages around (20 - 30) V and currents of a few
100 A, you have something like (2 - 10) kW/cm2 or more. Your
electrical range, for comparison, gets quite hot with just about 1/1000 of this
kind of power density.
So your electrode melts, and so does that part of the "parent" metal that is struck by the arc. Have your electrode made from the same material as the steel you want to weld, and you are in business, it seems.
|Not really. You can weld your steel, yes, but chances are that you are not going to be happy with the quality of the weld. For starters you should protect the surface of the liquid steel from contact with the air, as already mentioned above. The first measure for doing this is to use a "covered" electrode.|
|Early welders found
out that covering your steel wire electrode with paper, mud, concoctions from
tobacco stalks, and so on, might produce better welds. Not always, of course,
but often enough to indicate that a proper covering could be beneficial.
Nowadays we use three main kinds of coverings, mostly mixed with some powdered parent metal, too:
|What becomes clear is that welding is not as easy as it looks. If you consider to do some welding, it should be apparent that there are a lot of parameters that you must get just right. If you go for arc melting, you must pick the right electrode, the proper voltage and current, the right geometry, the right speed for moving the electrode along (always keeping the distance right), the proper pre-treatment of the parent metal (including, maybe, some pre-heating to temperatures above room temperature), and so on. If you got everything right, you might get a good-looking weld seam.|
|Now I can get to the crux of the welding problem: Even if you succeeded to produce a composition and microstructure of the weld seam (plus heat-affected zone) that is not too different from that of the parent metal, you still might be in in for major trouble: Your weld seam may develop cracks!|
|It goes without saying that this is deadly. If
your weld is cracking while you are still at it, you can just forget about it.
That is pretty bad but things can be even worse: your weld cracks after you finished it. Just about when the weld
finally reaches ambient temperature or - horror - a few days after the act!
There are several reasons for weld cracking, many related to hydrogen. And now we get to the more involved science, art and mysteries of welding. What, exactly, causes these cracks - and how can I avoid them?
|Welding and Crack Development|
|If cracks occur in your weld seam or
in the heat affected zone next to it, you know that you encountered fracture in
a nominally ductile material. I have given you three fracture modules already,
let's quickly recount the important points:
|"Normal" cracking can occur without the "help" of hydrogen. It often reveals itself as "center-line" or solidification cracking, and happens more or less shortly after solidification. This is what it might look like:|
|There are several reasons for this kind of
cracking to occur. First of all, there are always high stresses from the
thermal gradients. After solidification the hot parts shrink and then are under
tensile stress. If the center of the weld seam solidifies last as in the lower
of the two schematic drawings,
have enriched it with all kinds of impurities, and that typically makes a
material more brittle. Moreover, if the crystallites grow from the outside to
the center, the two crystallization fronts meet in the middle, possibly causing
a weak and porous
structure there for the reasons given in the link.
All of the above is tied to the geometry of your weld seam (or bead, as the experts call it). This is schematically illustrated above for two extreme solidification geometries.
Adjusting conditions (voltage power, geometry, ...) to "just right" values will allow to avoid the problem, particularly in mild steels.
There are some other "normal" cracks. They are mostly related to "bad" welding that produces, for example, slag inclusions or largish manganese sulfide precipitates, and I won't go into that.
| Let's now look at the real problem:
hydrogen-induced cracking. It comes under many names, e.g. hydrogen assisted cracking, heat affected zone cracking, cold cracking or delayed
Extremely simplified, what happens is that cracks develop in the heat affected zone (often close to the old solid-liquid interface) when it's "cold", i.e. the temperature is below about (150 100) °C ((200 - 300) °F). The susceptibility to hydrogen-induced cracking actually maximizes at about room temperature, and it may even take a day or two before these cracks develop.
Here is what it might look like:
|All this hydrogen related cracking is really bad, in particular because it get's worse for more advanced (high-strength) steels. Innumerous studies have been made and are being made since an outrageously large amount of money is tied to that. Consider that only one crack of this kind appears in the many thousands of welds in a 1000 mile long pipeline that is submerged in the Baltic. Repairing the pipeline will require serious money.|
|That's why the welding community came up with all kinds of empirical equations and graphs that relate weldability to composition. One example is shown below:|
|The figure is self-explaining and demonstrates
nicely that you run into serious welding problems with increasing carbon and
carbon-equivalent concentration. It
shows, for example, that plain steel with more than about 0.6 % carbon cannot
be welded. Here is one of the reasons why low-alloy steel is so popular.
The Graville diagram is, of course, just a guide and not always "true". Many more rules similar to the one embodied in this diagram exist - but I won't go into this since I do not intend to write another hyperscript, considerably longer than this one, about hydrogen and welding.
|Instead I will try to answer all your
questions that must have come up by now:
|The first question is the easiest one to answer. At the extreme temperatures and power density of the arc, hydrogen is produced from about anything that contains it. For example from organic stuff, like the cellulose that might cover the electrode, and in particular from water. Some water is always around; the water vapor contained in the air will already be enough to cause trouble. Even if you use electrodes covered with nominally hydrogen-free stuff (e.g. the basic electrode), it will have absorbed some water from the air. The surface of your steel also has a water vapor layer on it and possibly hydrogen containing oil, grease, dirt or paint, not to mention hydro-oxides called rust. You must bake your electrode for a while to drive out the water and clean and even pre-heat your steel and so on, if you want to minimize the amount of hydrogen produced during welding.|
|The second question also has an easy answer for
starters. Hydrogen does bad things because:
|What that means is that hydrogen at relevant
concentrations will get into the liquid part of the weld bead and from there
will diffuse into the heat affected zone and beyond. When the structure cools
down, hydrogen will become supersaturated and, since it is highly mobile,
always finds some defect where it can be absorbed. If that defect is a small
void or nanocrack - a dislocations pile-up might already do the trick -
something new happens. Two hydrogen atoms
might find room in there, engage in sex and firmly bond, forming a hydrogen
molecule (H2). This liberates a lot of energy and thus will happen
even if the crystal lattice has to be expanded a bit, i.e. even if the reaction
produces some elastic stress in the material. That stress attracts more
hydrogen atoms, and pretty soon there will be a nanocrack filled with hydrogen
molecules that is under high internal
pressure = stress.
Other hydrogen atoms may hang around dislocations, forming a kind of Cotrell-Bilby cloud. But in contrast to Cotrell-Bilby clouds formed by carbon or nitrogen interstitials, the dislocation can never outrun its groupies in this case; they are just too mobile. Dislocations enveloped in a hydrogen cloud thus will actually transport hydrogen over large distances as soon as they move in response to stress.
As soon as we look into details of all the stuff related above, things become cloudy. While there is no lack of studies made and papers written, there is still no full understanding of what exactly hydrogen does in iron (and other metals), and a lot of controversies among the scientists involved.
|When dealing with hydrogen it is best to forget everything about what interstitials normally do. Hydrogen just is not normal. It can do a lot of things (in particular if your steel contains all kinds of alloy elements and thus plenty of defects of all kinds), including a few special "quantum mechanical" ones, since it is so small. For example, it might diffuse by "tunneling", something normal atoms never do.|
|The third question is the tough one. In the relevant
literature more than five different mechanisms for hydrogen promoted cracking
are discussed. Some are mutually exclusive. For example, suggestions have been
made that hydrogen softens or hardens iron
/steel and that either mechanism somehow induces cracking.
It's time to point out that hydrogen-induced cracking or hydrogen embrittlement is not confined to just welding iron or steel but is a problem that plagues metallurgy in a rather broad context. Corrosion, for example, may produce hydrogen locally that diffuses into the steel along grain boundaries and helps to cause the sudden catastrophical collapse of large structures like the Berlin congress hall.
All I'm going to do now is to look at some of the things that could happen in the context of our basic equation for fracture:
|What the equation says is that as
soon as the critical stress is reached (at a nanocrack tip), fracture will
occur as long as the yield stress is higher than the critical stress. Hydrogen
thus can promote fracture by either lowering the critical stress and / or
raising the yield stress. It will already be bad enough if that happens only
So let's see what kind of mechanisms could do that, and how mechanisms discussed in the literature fit in with this concept
|The Hydrogen Induced
Decohesion Model says that dissolved hydrogen reduces the cohesive
strength of the lattice, i.e. the interatomic bond strength at a nanocrack tip
and thereby promotes decohesion. Since "interatomic bond strength" is
just another word for Young's modulus - Check! Could work.
If the hypothesis is true, the mechanism will bring down the critical stress for fracture.
|The Internal Pressure Model assumes that H2 formation in nanocracks, as pointed out above, produces high pressure inside these defects. The stress going with that is part of the critical stress, which is thus reached for lower external stress. Check once more! - could work.|
|The Surface Energy or Adsorption Model assumes that hydrogen is adsorpted at newly generated surfaces and then reduces the surface energy. The critical stress then comes down - Check once more! - could work.|
|The remainder of models deal with dislocations and hydrogen, and now it gets complicated. I will not even try to discuss this.|
|Suffice it to say that cracking during and after welding is a rather complex matter. To make things even more complicated, let's conceive that your weld did not develop cracks right away or after a few days. Does that mean that you are home-free now?|
|Of course not. Cracks may still develop
prematurely during re-heating, or in in
Well, if you are still with me and still considering to become a Material Scientist, congratulations! More timid persons have long since deserted to simpler occupations like banking + tax evasion or, like A. Merkel, to running a sizeable country.
|We have covered a lot of ground by now. Have you noticed how cunningly I evaded one of the more obvious questions concerning hydrogen-assisted cracking in welding? No? Well - here it is:|
|Why are those cracks typically found in the
heat-affected zone, quite often right at
the interface to the formerly liquid part, see
Well - I don't know. And neither, it seems, does anybody else. In all the papers and books that I consulted about this issue, the topic was evaded. I could make an educated guess, and lots of researchers, no doubt, have already done this, but a simple universally accepted explanation seems to be lacking.
The conclusion is obvious:
|We don't have a good welding theory yet. Let's hope that we will have one in the (near) future.|
General Remarks to Literature and Sources
Books and Other Major Sources
Fracture Mechanics I
Overview of Major Steels
9.2.2 Designing Low Alloy Steels
Spring Model and Properties of Crystals
Alloying Elements in Detail
Science of Alloying
Ductile to Brittle Transition or Cold Shortness
Diffusion in Iron
Overview of Major Steels: Scientific Steels
Riveting, Soldering, Liquid Welding Plus Gluing and Screwing
Overview of Major Steels: 1. Classifying Steels
Overview of Major Steels
Fracture Mechanics II
The Goldilocks Principle
Muliculti and Opera Singers
The Iron Carbon Phase Diagram
Segregation at Room Temperature
High Alloy Steels and Schäffler Diagram
© H. Föll (Iron, Steel and Swords script)